Effectiveness of Sugarcane Bagasse Ash (SCBA) as Partial Cement Replacement in
Mohd Khaidir ABU TALIB*, Noriyuki YASUFUKU**and Ryohei ISHIKURA***
(Received July 7, 2014)
Due to high organic content, presence of humic acid and less solid
particles in peat soil, cement alone is inadequate as a chemical admixture for this ground stabilization except a large quantity of cement is mixed.Sugarcane production is world number one commodities and produced a lot of bagasse.
Bagasse is burnt to generate power required for diverse activities in the factory and leave bagasse ash as a waste. Increasing concern of disposal of bagasse residual creates interest to explore the potential application of this material.
These research emphases on laboratory investigation on the application of sugarcane bagasse ash (SCBA) as partial cement replacement in peat
stabilization. Other than SCBA, calcium chloride (CaCl2), Ordinary Portland Cement (OPC) and silica sand (K7) were used as additives to stabilize the peat that sampled from Hokkaido, Japan. To develop the optimal mix design,
specimens of stabilized peat were tested in unconfined compression. Energy Dispersive X-ray (EDX) and Scanning Electron Microscope (SEM) apparatus
was used to examine elemental composition and microstructure. It was found that stabilized peat comprising 20% partial replacement of OPC with SCBA has
the maximum unconfined compressive strength (UCS) and discovered about 29 times greater than that of untreated peat specimen.
Keywords: Peat stabilization, Cement, Sugarcane bagasse ash, Unconfined compressive strength
Peat deposits distribution is extensive and can be found in many countries throughout the world when the conditions are favorable for their accumulation and formation1-3). The vastness of peat land coverage and its occurrence close to or within population centers and existing cropped areas
Graduate Student, Department of Civil and Structural Engineering **
Professor, Department of Civil Engineering ***
means some form of infrastructure development has to be carried out in these areas. To stimulate agriculture development for instance, basic civil engineering structures such as roads are required 4). Peat and organic soil represent the extreme form of soft soil and subject to instability and enormous primary as well as long-term settlement even when subjected to moderate load 5). These materials are very highly compressible together with very low shear strength 6).
The use of cement is not given much attention in the stabilization of organic soils because evasion is often become the first choice rather than build up any infrastructure on these problematic ground. However, over the past few years, there are researchers who began to observe the ability of the cement in the stabilization of organic soil6-12). It is well recognized that organic soils can retard or prevent the proper hydration of binders such as cement in binder-soil mixtures 9). Due to high organic content and less solid particles in peat soil, cement alone is insufficient as a chemical admixture for peat stabilization. That means unless a large quantity of cement is mixed with the soil to neutralize the acids, the process of the soil stabilization remains retarded. However, adding a large quantity of cement into the peat is definitely an unfriendly and uneconomical solution to deep peat ground improvement considering the fact that the peat ground is covers a wide area, and the rising cost of cement and its transportation to the site 13). Cement is responsible for about 5%–8% of global CO2 emissions and expected to grow 0.8 to 1.2% per year until may reach 4.4 billion tonnes of productions in 2050 14).
A pozzolana is a material occurring either naturally or artificially, and which contains silica, iron and aluminum ions that can generate a pozzolanic reaction 15). Small amount of pozzolans can be added to cement stabilized peat to enhance the secondary pozzolanic reaction in the stabilized soil 13) . One of pozzolan materials sources are getting from agricultural waste ash such as rice husk ash, straw ash and sugarcane bagasse ash. Production of large quantity of agricultural wastes all over the world faces serious problems of handling and disposal. The disposal of agricultural wastes creates a potential negative impact on the environment causing air pollution, water pollution finally affecting the local ecosystems. Hence safe disposal of agricultural wastes becomes challenging task for engineers 16).
Sugarcane production is world number one commodities with amount approximately 1.8 billion tonnes in 2012. Bagasse is the residue left after the crushing of sugar cane for juice extraction and on average about 32% of bagasse is produced from every tonne of sugar cane. Bagasse is burnt to generate power required for diverse activities in the factory and leave bagasse ash as a waste. Increasing concern of disposal of bagasse residual creates interest to explore the potential application of this material 17). The sugarcane industry is still seeking solutions to dispose of the wastes generated by the sugar and alcohol production processes. This ash is used as fertilizer in the plantations, but it does not have adequate mineral nutrients for this purpose. However, ash can be used in place of cement or sand in civil construction 18). Sugar cane bagasse ash (SCBA) has also been studied as a promising pozzolanic material. Nowadays, despite the increasing interest in the potential use of SCBA as a supplementary material of cement in concrete technology, there is no evidence in the current literature of its use in soil stabilization especially for organic soil.
2. Materials and experimental program
The materials that had been used are peat soil, Ordinary Portland Cement (OPC), silica sand so called K7, calcium chloride (CaCl2) and Sugarcane Bagasse Ash (SCBA). Peat samples were obtained from Sapporo in the Hokkaido region, Japan. For the purpose of laboratory experimental samples, peat was excavated approximately to a depth of 1 m below the ground surface. The SCBA samples were brought from Shinko Sugar Industry Co., Ltd, Kagoshima prefecture in Kyushu, Japan.
Other than OPC as main binder and CaCl2 as cement accelerator, well graded silica sand (K7) was prepared as a filler to increase the solid particles and enhance the filling effect of the stabilized peat. The entire laboratory test regulation and standards that had been implemented was shown in Table 1.
In order to understand the chemical reaction mechanism of mixture strengthening, an Energy Dispersive X-ray (EDX) had been conducted on untreated and treated peat and expected it will provide chemical evidence on the existence of calcium which is the major element of cementation products in the stabilized peat. In addition to such chemical characterization, the scanning electron micrographs are conducted to give micro visual evidence on cementation and void refinement of the stabilized soil.
The mix designs of stabilized peat for laboratory testing are shown in Table 2. The mix designs of stabilized peat were formulated in term of binder composition and dosage. Each binder dosage was determined based on the bulk density of peat at its average natural water content.
In producing each admixture, a mixer was used to intimately mix the peat with other materials for 10 minutes. Preparation of each test specimen of stabilized peat for unconfined compression test will be done by filling and tamping the stabilized soil admixture in five equal layers. Each cylinder mould has a size of 60 mm internal diameter and 300 mm height. The cylinder moulds then immersed in water for curing at specified duration under 20kPa initial pressure by using air pressure to simulate the surcharge pressure on the stabilized soil at site. After curing, the cylinder tube is removed and the test specimen is trimmed to the required size for testing. To evaluate the degree of improvement, the established parameters of the stabilized soil must be compared to those of untreated peat.
Table 1 Adopted standards for test method. Testing Names
Atterberg Limit JGS 0141-2009 Moisture Content ASTM- D 2974 Particle Size Distribution ASTM- D 422 Specific Gravity ASTM- D 854 Organic (ash) Content ASTM- D 2974 Fiber Content ASTM- D 1997 Acidity (pH Test) ASTM- D 2976 Unconfined Compression Strength ASTM- D 2166
3. Results and discussions
3.1 Materials Properties
Table 2 Laboratory mix design.
Type of test
Description of test purpose Curing durati on (days) OPC dosage (kgm-3)
Silica sand (K7) dosage (kgm-3)
Binder composition (abbreviation)
UCS* , pH, w**
To investigate the effect of binder composition on the
7 300 500 20
100% OPC (C100) 95%OPC:5%SCBA (C95B5) 90%OPC:10%SCB (C90B10) 85%OPC:15%SCB (C85B15) 80%OPC:20%SCB (C80B20) 75%OPC:25%SCB (C75B25) 70%OPC:30%SCB (C70B30) *
Unconfined Compressive Strength **
Table 3 Peat soil basic properties.
Peat soil properties Value
Natural water content, % 580
Ash content, % 16.79
Organic content , % 83.21
Bulk unit weight (kN/m3) 10.57 Specific gravity, Gs 1.67
Fiber content, % 43
Acidity ,pH 5.46
Liquid Limit, % 375
Compression Index, Cc 4.89
Undrained shear strength, kPa 6.8
Table 4 Oxide compounds of peat and materials.
CO2 86.78 - -
-NA2O 0.32 0.82 -
-MgO 0.38 1.26 0.18 1.69
P2O5 1.94 2.69 0.42 3.86
SO3 0.22 6.55 0.74 3.81
K2O 0.64 0.84 0.77 13.77
CaO 0.65 65.40 0.23 1.84
TiO2 0.62 - - 0.55
Al2O3 1.5 6.60 3.49 17.14
SiO2 5.48 10.26 93.52 51.61
Fe2O3 1.46 5.57 0.65 5.73
Al2O3+SiO2+Fe2O3 8.4 74.5
(%) Peat OPC
this study, OPC is predominantly characterized by 65.4% CaO, 10.26% SiO2, 6.6% Al2O3 and 5.57 Fe2O3. Based on a review, OPC is primarily characterized by quicklime (CaO), silica (SiO2), alumina (Al2O3) and ferric oxide (Fe2O3) 20). With a content of 93.52% SiO2, it can be affirmed that quartz is the major mineral in the silica sand.
For SCBA, it was found that the summation of the crucial pozzolanic oxide compounds (SiO2, Al2O3 and Fe2O3) is 74.5% of the total oxide compounds. These results indicate the suitability of SCBA as a pozzolan since the amount of such oxide compounds exceeds 70% as recommended by ASTM C 618 Standard.
The particle size distribution of the peat and other materials are tabulated in Fig. 1. The particle size distribution curves for the soils were obtained by dry sieve analysis. In addition to the normal sieve test method, the finer fraction was analyzed using a laser diffraction method (SALD). As can be seen, Hokkaido peat consists of 90% of the soil that finer than 4.75mm, and about 2% is finer than 75µm. Most of K7 particles sizes are 0.05 to 0.3mm in range while the size of SCBA particles consists more 80% finer than 0.045mm. According to ASTM C 618 Standard, volume fraction of more than 66% of particles smaller than 45 µm is required for a pozzolanic material.
Fig. 1 Particle size distribution of peat and materials.
3.2 Effect of partial replacement of OPC with SCBA
Figure 2 shows the experimental results of the effect of SCBA on the unconfined compressive strength of the stabilized peat. An optimal unconfined compressive strength of the stabilized soil was evaluated based on the results of unconfined compression tests on the specimens of stabilized peat with partial replacement of the cement with SCBA that varies from 5% to 35% as shown in Table 2.
Fig. 2 Effect of OPC-SCBA on the unconfined compressive strength of the untreated and treated peat.
Figure 2 also reveal that C100 mix composition is lower than calculated optimum mix composition (C80B20). The main reasons of this condition are because peat soil consists of high organic content and less solid particles as showing in Table 4. Organic soils can retard or prevent the proper hydration of binders such as cement in binder-soil mixtures and become insufficient to provide the desirable function for peat stabilization. Compared with clay and silt, peat has a considerably lower content of clay particles that can enter into secondary pozzolanic reactions 9, 21). The combination of humic acid with calcium ions produced in cement hydration makes it difficult for the calcium crystallization, which is responsible for the increase of peat soil-cement mixture strength to take place 10).
2 2 2 2
2 2 2 2
3 .2 .3 ( ) (1)
( ) 3 .2 .3 (2)
Cement H O CaO SiO H O Ca OH
Ca OH Pozzolan H O CaO SiO H O
+ = + − − − − − −
+ + = − − − − −
The general chemical reactions between cement and pozzolan with water are denoted in Equations 1 and 2. Calcium silicate hydrate or also known as tobermorite gels (3CaO.2SiO2.3H2O) are formed when cement reacts with water in peat. This gel act as adhesive that binds and grasp the soil particles together. Nevertheless, humic acid in peat reacts with calcium ion to form insoluble calcium humid acid. These conditions make the secondary pozzolanic reaction between calcium hydroxide (Ca (OH) 2) and the peat is inhibited and this renders a low strength gain in the soil-cement mixture.
probable because the pozzolan which contains extra silica and alumina that activated by cement is able to counterbalance the acid and create an alkaline atmosphere that boosts the secondary pozzolanic reaction within the cemented soil. Additional secondary tobermorite gels densify the stabilized peat, thereby further enhancing its strength13).
Generally, the pozzolanic effect depends not only on the pozzolanic reaction but also on the physical or filler effect of the smaller particles in the mixture 20). The positive result indicates that the optimal mix design can be effectively applied to stabilize the peat in such a way that the fine particles of pozzolan fill up the pore spaces of the cemented soil, thus closely packing, reinforcing and strengthening its matrix as the hydration and pozzolanic products are formed during cement hydrolysis 22).
Figure 3 depicts the results of Scanning Electron Microscope (SEM) on untreated and some treated peat samples. Obvious change had seen and occurred when comparing the SEM results of stabilized peat with the untreated peat. It has been observed that the untreated peat consists of coarse organic particles and fibers in a loose condition. They were organized arbitrarily without significant microstructural orientation. The organic coarse particles were typically hollow and spongy. Due to spongy nature of organic coarse particles, untreated peat is highly compressible and has a high water holding capacity when fully saturated23).
Fig. 3 Scanning Electron Microscope (SEM) on untreated and treated peat.
Minor void spaces can be detected in the photomicrographs of stabilized peats mixtures (C100, C80B20 and C70B30). Compared to C100 and C70B30 mixtures, a C80B20 mixture gave the significant pore improvement that can be perceived in the photomicrograph of the stabilized peat. It can be stated that the stabilized soil is characterized by a well cemented soil medium with tiny pore spaces within it as a result of the pozzolanic activity of SCBA.
minerals was involved in the secondary pozzolan reaction that boosted by more calcium hydroxide [Ca (OH) 2]. At mix binder C70B30, carbon (CO2) and main pozzolanic minerals (SiO2, Al2O3 and Fe2O3) illustrates the increment value while the calcium (CaO) oxide was declining. These occurrences happened because when insufficient cement is added, hydration and pozzolanic reaction become lower and effective neutralization of humid acids within the soil is not achieved. This is due to the limited formation of primary cementation products to bind the soil because the soil organic matter tends to retain the calcium ions produced from cement hydrolysis, resulting in a limited amount of calcium hydroxide [Ca (OH) 2] that could react with silica (SiO2) and alumina (Al2O3) of SCBA to yield secondary pozzolanic products during the pozzolanic reaction.
Table 5 Energy Dispersive X-ray (EDX) test results of untreated and treated peat.
CO2 78.86 ± 7.92 8.76 ± 2.90 5.17 ± 1.24 25.88 ± 2.33
NA2O 0.32 ± 0.01 0.15 ± 0.02 0.26 ± 0.08 0.32 ± 0.08
MgO 0.63 ± 0.25 0.64 ± 0.10 0.98 ± 0.33 0.96 ± 0.40
Al2O3 2.95 ± 1.45 5.64 ± 1.19 4.92 ± 0.09 6.63 ± 0.14
SiO2 9.55 ± 4.07 24.21 ± 6.68 17.21 ± 1.22 23.63 ± 0.8
P2O5 2.33 ± 0.39 1.38 ± 0.06 2.83 ± 0.00 1.26 ± 0.35
SO3 0.22 ± 0.00 1.36 ± 0.06 2.97 ± 1.69 2.42 ± 0.02
K2O 0.92 ± 0.28 2.26 ± 0.34 2.77 ± 0.64 4.48 ± 0.27 CaO 0.43 ± 0.23 51.09 ± 3.94 56.72 ± 4.7 30.14 ± 0.88 TiO2 0.89 ± 0.23 1.35 ± 0.05 2.29 ± 0.62 0.76 ± 0.02 Fe2O3 3.04 ± 1.58 3.19 ± 1.4 3.92 ± 2.06 3.55 ± 0.10 Al2O3+SiO2+Fe2O3 15.54 ± 7.1 33.04 ± 9.27 26.05 ± 3.37 33.81 ± 1.04
Oxide Compound Untreated Peat, %
Stabilized Peat, %
C100 C80B20 C70B30
Utilization of sugarcane bagasse ash (SCBA) as partial cement replacement in peat stabilization has been examined. It can be summarized from the experimental results that SCBA has made a significant influence on the physical, mechanical and chemical properties of the stabilized peat. Based on the outcome of the laboratory analysis, the following concluding comments are made.
i. Untreated peat in this study can be classified as hemic peat with high ash content and moderate acidic. With the high water content, high liquid limit and low shear strength, this soil demonstrated the high compressibility and instability characteristics.
ii. It was found that the summation of the vital pozzolanic oxide compounds (SiO2, Al2O3 and Fe2O3) for SCBA that had been used is 74.5% of the total oxide compounds which is indicate the suitability of this materials as a pozzolan since the amount of such oxide compounds exceeds 70% as recommended by ASTM C 618 Standard.
iv. Compared to untreated soil, SEM results for stabilized peat gave the significant pore improvement that can be perceived in the photomicrograph and it can be stated that the stabilized soil is characterized by a well cemented soil medium with small pore spaces within it as a result of the pozzolanic activity of SCBA.
v. EDX results prove that the lower carbon (CO2) and higher calcium (CaO) oxide fractions will gave the better results of strength.
Overall, it is suggested that the obtained optimum mix design can be applied to stabilize the shallow peat layer in order to support road embankment for low to medium-volume road.
The authors would like to thank Shinko Sugar Industry Co. Ltd for provide sugarcane bagasse ash, Mr. Michio Nakashima for technical assistance and all members of Kyushu University Geotechnical Laboratory for their supports.
1) Asadi, A.,Huat, B.B.K.,Hanafi, M.M.,Mohamed, T.A. and Shariatmadari, N., 2009. Role of organic matter on electroosmotic properties and ionic modification of organic soils. Geosciences Journal, 13(2): 175-181.
2) Duraisamy, Y.,Huat, B.K.,Muniandy, R. and Aziz, A.A., 2008. Compressibility Behavior of Fibrous Peat Reinforced with Cement Columns. ICCBT- E- (09)–pp93-110.
3) Montanarella, L.,Jones, R.J.A. and Hiederer, 2006. The distribution of peatland in Europe. Mires and Peat, 1 (2006), Article 01, 1-10.
4) Huat, B.K.,Sew, G.S. and Ali, F.H., 2004. Organic and Peat Soils Engineering. Serdang, University Putra Malaysia, Press, ISBN Number: 983-2871-08-5.
5) Jarrett, P.M., 1995. Site investigation for organic soils and peat. Geoguide 6. JKR Document 20709- 0341-95. Public Works Department Malaysia. Malaysia.
6) Huat, B.K.,Maail, S. and Mohamed, T.A., 2005. Effect of Chemical Admixtures on the Engineering Properties of Tropical Peat Soils. American Journal of Applied Sciences, 2(7): 1113-1120.
7) EuroSoilStab, 2002. Development of design and construction methods to stabilize soft organic soils. Design guide soft soil stabilization. CT97-0351. Project No. BE 96-3177, Industrial & Materials TechnologiesProgramme (Brite- EuRam III), European Commission.
8) Axelsson, K.,Johansson, S.E. and Anderson, R., 2002. Stabilization of Organic Soils by Cement and Puzzolanic Reactions- Feasibility Study, Swedish deep stabilization Research Centre, Report 3, English translation.
9) Hebib, S. and Farrell, E.R., 2003. Some experiences on the stabilization of Irish peats. Canadian Geotechnical Journal, 40(1): 107-120.
10) Chen, H. and Wang, Q., 2006. The behaviour of organic matter in the process of soft soil stabilization using cement. Bulletin of Engineering Geology and the Environment, 65(4): 445-448.
12) Ahnberg, H., 2006. Strength of stabilised soils– A laboratory study on clays and organic soils stabilised with different types of binder, Swedish deep stabilization Research Centre, Report 16, English translation.
13) Wong, L.S.,Hashim, R. and Ali, F.H., 2009. A Review on Experimental Investigations of Peat Stabilization. Australian Journal of Basic and Applied Sciences, 3(4): 3537-3552, 2009. ISSN 1991-8178.
14) World Business Council for Sustainable Development, W.B.C.S.D. and International Energy Agency, I.E.A., 2009. Cement Technology Roadmap 2009.
15) Velosa, A.L. and Cachim, P.B., 2009. Hydraulic-lime based concrete: Strength development using a pozzolanic addition and different curing conditions. Construction and Building Materials, 23(5): 2107-2111.
16) Chittaranjan, M.,Vijay, M. and Keerthi, D., 2011. Agricultural wastes as soil stabilizers International Journal of Earth Sciences and Engineering, ISSN 0974-5904, Volume 04, No 06 SPL, October 2011, pp 50-51
17) Lee, S.C. and Mariatti, M., 2008. The effect of bagasse fibers obtained (from rind and pith component) on the properties of unsaturated polyester composites. Materials Letters, 62(16): 2253-2256.
18) Cordeiro, G.C.,Toledo Filho, R.D.,Tavares, L.M. and Fairbairn, E.M.R., 2009. Ultraﬁne grinding of sugar cane bagasse ash for application as pozzolanic admixture in concrete. Cement and Concrete Research 39, 110-115.
19) ASTM, 2000. American Society of Testing Materials, Annual Book of ASTM Standards, Section four: Construction, vol. 04.08.
20) Isaia, G.C.,Gastaldini, A.L.G. and Moraes, R., 2003. Physical and pozzolanic action of mineral additions on the mechanical strength of high-performance concrete. Cement & Concrete Composites, 25(1): 69-76.
21) Janz, M. and Johansson, S.E., 2002. The function of different binding agents in deep stabilization, Swedish Deep Stabilization Research Center, Linkoping: SGI. 9.
22) Wong, L.S.,Hashim, R. and Ali, F., 2013. Utilization of sodium bentonite to maximize the filler and pozzolanic effects of stabilized peat. Engineering Geology, 152(1): 56-66. 23) Wong, L.S.,Hashim, R. and Ali, F., 2013. Improved strength and reduced permeability of
stabilized peat: Focus on application of kaolin as a pozzolanic additive. Construction and Building Materials, 40: 783-792.